| IUPAC name |
|Other names |
Titanium Sulfide, titanium sulphide, titanium disulfide, titanium disulphide
3D model (JSmol)
CompTox Dashboard (EPA)
|Molar mass||111.997 g/mol|
|Density||3.22 g/cm3, solid|
|hexagonal, space group P3m1, No. 164|
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
(what is ?)
Titanium disulfide is an inorganic compound with the formula Ti S 2. A golden yellow solid with high electrical conductivity,it belongs to a group of compounds called transition metal dichalcogenides, which consist of the stoichiometry M E 2. TiS2 has been employed as a cathode material in rechargeable batteries.
With a layered structure, TiS2 adopts a hexagonal close packed (hcp) structure, analogous to cadmium iodide (CdI2). In this motif, half of the octahedral holes are filled with a "cation", in this case Ti4+. 3m1. The Ti-S bond lengths are 2.423 Å.Each Ti centre is surrounded by six sulfide ligands in an octahedral structure. Each sulfide is connected to three Ti centres, the geometry at S being pyramidal. Several metal dichalcogenides adopt similar structures, but some, notably MoS2, do not. The layers of TiS2 consist of covalent Ti-S bonds. The individual layers of TiS2 are bound together by van der Waals forces, which are relatively weak intermolecular forces. It crystallises in the space group P
The single most useful and most studied property of TiS2 is its ability to undergo intercalation upon treatment with electropositive elements. The process is a redox reaction, illustrated in the case of lithium:
LiTiS2 is generally described as Li+[TiS2−]. During the intercalation and deintercalation, a range of stoichimetries are produced with the general formul LixTiS2 (x < 1). During intercalation, the interlayer spacing expands (the lattice "swells") and the electrical conductivity of the material increases. Intercalation is facilitated because of the weakness of the interlayer forces as well as the susceptibility of the Ti(IV) centers toward reduction. Intercalation can be conducted by combining a suspension of the disulfide material and a solution of the alkali metal in anhydrous ammonia. Alternatively solid TiS2 reacts with the alkali metal upon heating.
The Rigid-Band Model (RBM), which assumes that electronic band structure does not change with intercalation, describes changes in the electronic properties upon intercalation.
Deintercalation is the opposite of intercalation; the cations diffuse out from between the layers. This process is associated with recharging a Li/TiS2 battery. Intercalation and deintercalation can be monitored by cyclic voltammetry. The microstructure of the titanium disulfide greatly affects the intercalation and deintercalation kinetics. Titanium disulfide nanotubes have a higher uptake and discharge capacity than the polycrystalline structure.The higher surface area of the nanotubes is postulated to provide more binding sites for the anode ions than the polycrystalline structure.
Formally containing the d0 ion Ti4+ and closed shell dianion S2−, TiS2 is essentially diamagnetic. Its magnetic susceptibility is 9 x 10−6 emu/mol, the value being sensitive to stoichiometry.Titanium disulfide is a semimetal, meaning there is small overlap of the conduction band and valence band.
The properties of titanium disulfide powder have been studied by high pressure synchrotron x-ray diffraction (XRD) at room temperature.At ambient pressure, TiS2 behaves as semiconductor while at high pressures of 8 GPa the material behaves as a semimetal. At 15 GPa, the transport properties change. There is no significant change in the density of states at the Fermi level up to 20 GPa and phase change does not occur until 20.7 GPa. A change in the structure of TiS2 was observed at a pressure of 26.3 GPa, although the new structure of the high pressure phase has not been determined.
The unit cell of titanium disulfide is 3.407 by 5.695 angstroms. The size of the unit cell decreased at 17.8 GPa. The decrease in unit cell size was greater than was observed for MoS2 and WS2, indicating that titanium disulfide is softer and more compressible. The compression behavior of titanium disulfide is anisotropic. The axis parallel to S-Ti-S layers (c-axis) is more compressible than the axis perpendicular to S-Ti-S layers (a-axis) because of weak van der waals forces keeping S and Ti atoms together. At 17.8 GPa, the c-axis is compressed by 9.5% and the a-axis is compressed by 4%. The longitudinal sound velocity is 5284 m/s in the plane parallel to S-Ti-S layers. The longitudinal sound velocity perpendicular to the layers is 4383 m/s.
Titanium disulfide is prepared by the reaction of the elements around 500 °C.
It can be more easily synthesized from titanium tetrachloride, but this product is typically less pure than that obtained from the elements.
This route has been applied to the formation of TiS2 films by chemical vapor deposition. Thiols and organic disulfides can be employed in place of hydrogen sulfide.
A variety of other titanium sulfides are known.
Samples of TiS2 are unstable in air.Upon heating, the solid undergoes oxidation to titanium dioxide:
TiS2 is also sensitive to water:
Upon heating, TiS2 releases sulfur, forming the titanium(III) derivative:
Thin films of TiS2 have been prepared by the sol-gel process from titanium isopropoxide (Ti(OPri)4) followed by spin coating.This method affords amorphous material that crystallised at high temperatures to hexagonal TiS2, which crystallization orientations in the , , and  directions. Because of their high surface area, such films are attractive for battery applications.
More specialized morphologies—nanotubes, nanoclusters, whiskers, nanodisks, thin films, fullerenes—are prepared by combining the standard reagents, often TiCl4 in unusual ways. For example, flower-like morphologies were obtain by treating a solution of sulfur in 1-octadecene with titanium tetrachloride.
A form of TiS2 with a fullerene-like structure has been prepared using the TiCl4/H2S method. The resulting spherical structures have diameters between 30 and 80 nm. Owing to their spherical shape, these fullerenes exhibit reduced friction coefficient and wear, which may prove useful in various applications.
Nanotubes of TiS2 can be synthesized using a variation of the TiCl4/H2S route. According to transmission electron microscopy (TEM), these tubes have an outer diameter of 20 nm and an inner diameter of 10 nm. The average length of the nanotubes was 2-5 µm and the nanotubes were proven to be hollow. TiS2 nanotubes with open ended tips are reported to store up to 2.5 weight percent hydrogen at 25 °C and 4 MPa hydrogen gas pressure. Absorption and desorption rates are fast, which is an attractive for hydrogen storage. The hydrogen atoms are postulated to bind to sulfur.
Nanoclusters, or quantum dots of TiS2 have distinctive electronic and chemical properties due to quantum confinement and very large surface to volume ratios. Nanoclusters can be synthesized using micelle. The nanoclusters are prepared from a solution of TiCl4 in tridodecylmethyl ammonium iodide (TDAI), which served as the inverse micelle structure and seeded the growth of nanoclusters in the same general reaction as nanotubes.Nucleation only occurs inside the micelle cage due to the insolubility of the charged species in the continuous medium, which is generally a low dielectric constant inert oil. Like the bulk material, nanocluster-form of TiS2 is a hexagonal layered structure. . Quantum confinement creates well separated electronic states and increases the band gap more than 1 eV in comparison to the bulk material. A spectroscopic comparison shows a large blueshift for the quantum dots of 0.85 eV.
Nanodisks of TiS2 arise by treating TiCl4 with sulfur in oleylamine.
The promise of titanium disulfide as a cathode material in rechargeable batteries was described in 1973 by M. Stanley Whittingham.The Group IV and V dichalcogenides attracted attention for their high electrical conductivities. The originally described battery used a lithium anode and a titanium disulfide cathode. This battery had high energy density and the diffusion of lithium ions into the titanium disulfide cathode was reversible, making the battery rechargeable. Titanium disulfide was chosen because it is the lightest and cheapest chalcogenide. Titanium disulfide also has the fastest rate of lithium ion diffusion into the crystal lattice. The main problem was degradation of the cathode after multiple recycles. This reversible intercalation process allows the battery to be rechargeable. Additionally, titanium disulfide is the lightest and the cheapest of all group IV and V layered dichalcogenides. In the 1990s, titanium disulfide was replaced by other cathode materials (manganese and cobalt oxides) in most rechargeable batteries.
The use of TiS2 cathodes remains of interest for use in solid-state lithium batteries, e.g., for hybrid electric vehicles and plug-in electric vehicles.
In contrast to the all-solid state batteries, most lithium batteries employ liquid electrolytes, which pose safety issues due to their flammability. Many different solid electrolytes have been proposed to replace these hazardous liquid electrolytes. For most solid-state batteries, high interfacial resistance lowers the reversibility of the intercalation process, shortening the life cycle. These undesirable interfacial effects are less problematic for TiS2. One all-solid-state lithium battery exhibited a power density of 1000 W/kg over 50 cycles with a maximum power density of 1500 W/kg. Additionally, the average capacity of the battery decreased by less than 10% over 50 cycles. Although titanium disulfide has high electrical conductivity, high energy density, and high power, its discharge voltage is relatively low compared to other lithium batteries where the cathodes have higher reduction potentials.
A lithium-ion or Li-ion battery is a type of rechargeable battery which uses the reversible reduction of lithium ions to store energy. It is the predominant battery type used in portable consumer electronics and electric vehicles. It also sees significant use for grid-scale energy storage and military and aerospace applications. Compared to other rechargeable battery technologies, Li-ion batteries have high energy densities, low self-discharge, and no memory effect.
Molybdenum disulfide is an inorganic compound composed of molybdenum and sulfur. Its chemical formula is MoS
In chemistry, intercalation is the reversible inclusion or insertion of a molecule into layered materials with layered structures. Examples are found in graphite and transition metal dichalcogenides.
A chalcogenide is a chemical compound consisting of at least one chalcogen anion and at least one more electropositive element. Although all group 16 elements of the periodic table are defined as chalcogens, the term chalcogenide is more commonly reserved for sulfides, selenides, tellurides, and polonides, rather than oxides. Many metal ores exist as chalcogenides. Photoconductive chalcogenide glasses are used in xerography. Some pigments and catalysts are also based on chalcogenides. The metal dichalcogenide MoS2 is a common solid lubricant.
Tungsten disulfide is an inorganic chemical compound composed of tungsten and sulfur with the chemical formula WS2. This compound is part of the group of materials called the transition metal dichalcogenides. It occurs naturally as the rare mineral tungstenite. This material is a component of certain catalysts used for hydrodesulfurization and hydrodenitrification.
Michael Stanley Whittingham is a British-American chemist. He is currently a professor of chemistry and director of both the Institute for Materials Research and the Materials Science and Engineering program at Binghamton University, State University of New York. He also serves as director of the Northeastern Center for Chemical Energy Storage (NECCES) of the U.S. Department of Energy at Binghamton. He was awarded the Nobel Prize in Chemistry in 2019 alongside Akira Yoshino and John B. Goodenough.
Nanobatteries are fabricated batteries employing technology at the nanoscale, particles that measure less than 100 nanometers or 10−7 meters. These batteries may be nano in size or may use nanotechnology in a macro scale battery. Nanoscale batteries can be combined to function as a macrobattery such as within a nanopore battery.
Lithium cobalt oxide, sometimes called lithium cobaltate or lithium cobaltite, is a chemical compound with formula LiCoO
2. The cobalt atoms are formally in the +3 oxidation state, hence the IUPAC name lithium cobalt(III) oxide.
A lithium-ion capacitor (LIC) is a hybrid type of capacitor classified as a type of supercapacitor. It is called a hybrid because the anode is the same as those used in lithium-ion batteries and the cathode is the same as those used in supercapacitors. Activated carbon is typically used as the cathode. The anode of the LIC consists of carbon material which is often pre-doped with lithium ions. This pre-doping process lowers the potential of the anode and allows a relatively high output voltage compared to other supercapacitors.
Lithium titanates are chemical compounds of lithium, titanium and oxygen. They are mixed oxides and belong to the titanates. The most important lithium titanates are:
The lithium–air battery (Li–air) is a metal–air electrochemical cell or battery chemistry that uses oxidation of lithium at the anode and reduction of oxygen at the cathode to induce a current flow.
A potassium-ion battery or K-ion battery is a type of battery and analogue to lithium-ion batteries, using potassium ions for charge transfer instead of lithium ions. It was invented by the Iranian/American chemist Ali Eftekhari in 2004.
Graphene foam is a solid, open-cell foam made of single-layer sheets of graphene. It is a candidate substrate for the electrode of lithium-ion batteries.
Titanium diselenide (TiSe2) also known as titanium(IV) selenide, is an inorganic compound of titanium and selenium. In this material selenium is viewed as selenide (Se2−) which requires that titanium exists as Ti4+. Titanium diselenide is a member of metal dichalcogenides, compounds that consist of a metal and an element of the chalcogen column within the periodic table. Many exhibit properties of potential value in battery technology, such as intercalation and electrical conductivity, although most applications focus on the less toxic and lighter disulfides, e.g. TiS2.
A lithium ion manganese oxide battery (LMO) is a lithium-ion cell that uses manganese dioxide, MnO
2, as the cathode material. They function through the same intercalation/de-intercalation mechanism as other commercialized secondary battery technologies, such as LiCoO
2. Cathodes based on manganese-oxide components are earth-abundant, inexpensive, non-toxic, and provide better thermal stability.
Research in lithium-ion batteries has produced many proposed refinements of lithium-ion batteries. Areas of research interest have focused on improving energy density, safety, rate capability, cycle durability, flexibility, and cost.
Magnesium batteries are batteries that utilize magnesium cations as the active charge transporting agents in solution and often as the elemental anode of an electrochemical cell. Both non-rechargeable primary cell and rechargeable secondary cell chemistries have been investigated. Magnesium primary cell batteries have been commercialised and have found use as reserve and general use batteries.
Calcium (ion) batteries are energy storage and delivery technologies (i.e., electro–chemical energy storage) that employ calcium ions (cations), Ca2+, as the active charge carrier in the electrolytes as well as in the electrodes (anode and cathode). Calcium (ion) batteries remain an active area of research, with studies and work persisting in the discovery and development of electrodes and electrolytes that enable stable, long-term battery operation.
In material science, layered materials are solids with highly anisotropic bonding, in which two-dimensional sheets are internally strongly bonded, but only weakly bonded to adjacent layers. Owing to their distinctive structures, layered materials are often suitable for intercalation reactions.
This is a history of the lithium-ion battery.